# Electronic Supplementary Material (ESI) for RSC Advances.
# This journal is © The Royal Society of Chemistry 2014

#######################################################################
#
#                 Cambridge Crystallographic Data Centre
#                                CCDC 
# 
#######################################################################
# 
#  This CIF contains data from an original supplementary publication
#  deposited with the CCDC, and may include chemical, crystal,
#  experimental, refinement, atomic coordinates,
#  anisotropic displacement parameters and molecular geometry data,
#  as required by the journal to which it was submitted.
#
#  This CIF is provided on the understanding that it is used for bona
#  fide research purposes only. It may contain copyright material
#  of the CCDC or of third parties, and may not be copied or further
#  disseminated in any form, whether machine-readable or not,
#  except for the purpose of generating routine backup copies
#  on your local computer system.
# 
#  For further information on the CCDC, data deposition and
#  data retrieval see:
#                         www.ccdc.cam.ac.uk
#
#  Bona fide researchers may freely download Mercury and enCIFer
#  from this site to visualise CIF-encoded structures and 
#  to carry out CIF format checking respectively.
#
data_3333

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Ca Cs4 F12 Mg3'
_chemical_formula_weight         872.65

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           trigonal
_symmetry_space_group_name_H-M   R-3m

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'-x, -x+y, -z'
'x-y, -y, -z'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+1/3'
'-x+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, -y+1/3, -z+1/3'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+2/3'
'-x+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, -y+2/3, -z+2/3'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'x, x-y, z'
'-x+y, y, z'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z+1/3'
'x+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, y+1/3, z+1/3'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+2/3'
'x+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, y+2/3, z+2/3'

_cell_length_a                   6.2196(9)
_cell_length_b                   6.2196(9)
_cell_length_c                   29.812(9)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_volume                     998.7(4)
_cell_formula_units_Z            3
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    1531
_cell_measurement_theta_min      3.84
_cell_measurement_theta_max      27.54

_exptl_crystal_description       block
_exptl_crystal_colour            colorless
_exptl_crystal_size_max          0.145
_exptl_crystal_size_mid          0.13
_exptl_crystal_size_min          0.097
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.353
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1152
_exptl_absorpt_coefficient_mu    11.512
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_correction_T_min  0.645
_exptl_absorpt_correction_T_max  0.746
_exptl_absorpt_process_details   face-indexed

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         0
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            2049
_diffrn_reflns_av_R_equivalents  0.0183
_diffrn_reflns_av_sigmaI/netI    0.0112
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_l_min       -38
_diffrn_reflns_limit_l_max       37
_diffrn_reflns_theta_min         3.84
_diffrn_reflns_theta_max         27.56
_reflns_number_total             329
_reflns_number_gt                313
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       'Bruker APEX2'
_computing_cell_refinement       'Bruker SAINT'
_computing_data_reduction        'Bruker SAINT'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0087P)²+3.0175P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   ?
_refine_ls_hydrogen_treatment    ?
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.00103(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         329
_refine_ls_number_parameters     27
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0123
_refine_ls_R_factor_gt           0.0110
_refine_ls_wR_factor_ref         0.0256
_refine_ls_wR_factor_gt          0.0247
_refine_ls_goodness_of_fit_ref   1.202
_refine_ls_restrained_S_all      1.202
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cs1 Cs 0.0000 0.0000 0.131513(10) 0.01625(11) Uani 1 6 d S . .
Cs2 Cs 0.6667 0.3333 0.050278(10) 0.01415(11) Uani 1 6 d S . .
Mg1 Mg 0.3333 0.6667 0.1667 0.0110(5) Uani 1 12 d S . .
Mg2 Mg 0.3333 0.6667 0.07507(5) 0.0102(3) Uani 1 6 d S . .
Ca1 Ca 0.0000 0.0000 0.0000 0.0114(3) Uani 1 12 d S . .
F1 F 0.17524(15) 0.3505(3) 0.04161(5) 0.0173(4) Uani 1 2 d S . .
F2 F 0.0570(3) 0.52851(15) 0.12313(5) 0.0149(4) Uani 1 2 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cs1 F2 3.1349(5) 2 ?
Cs1 F2 3.1349(5) . ?
Cs1 F2 3.1349(5) 3 ?
Cs1 F2 3.1349(5) 2_665 ?
Cs1 F2 3.1349(5) 3_455 ?
Cs1 F2 3.1349(5) 1_545 ?
Cs1 F2 3.1503(17) 26_445 ?
Cs1 F2 3.1503(17) 27 ?
Cs1 F2 3.1503(17) 25_455 ?
Cs1 F1 3.2783(18) 2 ?
Cs1 F1 3.2783(18) 3 ?
Cs1 F1 3.2783(18) . ?
Cs2 F2 3.0229(16) 1_655 ?
Cs2 F2 3.0229(16) 3 ?
Cs2 F2 3.0229(16) 2_665 ?
Cs2 F1 3.1219(5) 2_655 ?
Cs2 F1 3.1219(5) 1_655 ?
Cs2 F1 3.1219(5) 3 ?
Cs2 F1 3.1219(5) 3_665 ?
Cs2 F1 3.1219(5) . ?
Cs2 F1 3.1219(5) 2_665 ?
Cs2 F1 3.2256(18) 21_655 ?
Cs2 F1 3.2256(18) 20 ?
Cs2 F1 3.2256(18) 19_665 ?
Mg1 F2 1.9747(16) . ?
Mg1 F2 1.9747(16) 3_565 ?
Mg1 F2 1.9747(16) 2_665 ?
Mg1 F2 1.9747(16) 25_565 ?
Mg1 F2 1.9747(16) 27 ?
Mg1 F2 1.9748(16) 26_455 ?
Mg2 F1 1.9737(18) 3_565 ?
Mg2 F1 1.9737(18) . ?
Mg2 F1 1.9737(18) 2_665 ?
Mg2 F2 2.066(2) 3_565 ?
Mg2 F2 2.066(2) . ?
Mg2 F2 2.066(2) 2_665 ?
Ca1 F1 2.2589(16) 19 ?
Ca1 F1 2.2589(16) . ?
Ca1 F1 2.2589(16) 21 ?
Ca1 F1 2.2589(16) 3 ?
Ca1 F1 2.2589(16) 20 ?
Ca1 F1 2.2589(16) 2 ?
F1 Cs2 3.1219(5) 1_455 ?
F1 Cs2 3.2256(18) 19_665 ?
F2 Cs2 3.0229(16) 1_455 ?
F2 Cs1 3.1349(5) 1_565 ?
F2 Cs1 3.1503(17) 25_455 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F2 Cs1 F2 119.371(8) 2 . ?
F2 Cs1 F2 119.371(8) 2 3 ?
F2 Cs1 F2 119.371(8) . 3 ?
F2 Cs1 F2 165.49(6) 2 2_665 ?
F2 Cs1 F2 48.55(6) . 2_665 ?
F2 Cs1 F2 71.02(6) 3 2_665 ?
F2 Cs1 F2 48.55(6) 2 3_455 ?
F2 Cs1 F2 71.02(6) . 3_455 ?
F2 Cs1 F2 165.49(6) 3 3_455 ?
F2 Cs1 F2 119.371(8) 2_665 3_455 ?
F2 Cs1 F2 71.02(6) 2 1_545 ?
F2 Cs1 F2 165.49(6) . 1_545 ?
F2 Cs1 F2 48.55(6) 3 1_545 ?
F2 Cs1 F2 119.371(8) 2_665 1_545 ?
F2 Cs1 F2 119.371(8) 3_455 1_545 ?
F2 Cs1 F2 97.17(3) 2 26_445 ?
F2 Cs1 F2 126.873(15) . 26_445 ?
F2 Cs1 F2 56.86(5) 3 26_445 ?
F2 Cs1 F2 97.17(3) 2_665 26_445 ?
F2 Cs1 F2 126.873(15) 3_455 26_445 ?
F2 Cs1 F2 56.86(5) 1_545 26_445 ?
F2 Cs1 F2 126.873(15) 2 27 ?
F2 Cs1 F2 56.86(5) . 27 ?
F2 Cs1 F2 97.17(3) 3 27 ?
F2 Cs1 F2 56.86(5) 2_665 27 ?
F2 Cs1 F2 97.17(3) 3_455 27 ?
F2 Cs1 F2 126.873(15) 1_545 27 ?
F2 Cs1 F2 70.62(5) 26_445 27 ?
F2 Cs1 F2 56.86(5) 2 25_455 ?
F2 Cs1 F2 97.17(3) . 25_455 ?
F2 Cs1 F2 126.873(15) 3 25_455 ?
F2 Cs1 F2 126.873(15) 2_665 25_455 ?
F2 Cs1 F2 56.86(5) 3_455 25_455 ?
F2 Cs1 F2 97.17(3) 1_545 25_455 ?
F2 Cs1 F2 70.62(5) 26_445 25_455 ?
F2 Cs1 F2 70.62(5) 27 25_455 ?
F2 Cs1 F1 53.98(4) 2 2 ?
F2 Cs1 F1 89.50(3) . 2 ?
F2 Cs1 F1 113.66(4) 3 2 ?
F2 Cs1 F1 113.66(4) 2_665 2 ?
F2 Cs1 F1 53.98(4) 3_455 2 ?
F2 Cs1 F1 89.50(3) 1_545 2 ?
F2 Cs1 F1 143.224(19) 26_445 2 ?
F2 Cs1 F1 143.223(19) 27 2 ?
F2 Cs1 F1 102.97(4) 25_455 2 ?
F2 Cs1 F1 89.50(3) 2 3 ?
F2 Cs1 F1 113.66(4) . 3 ?
F2 Cs1 F1 53.98(4) 3 3 ?
F2 Cs1 F1 89.50(3) 2_665 3 ?
F2 Cs1 F1 113.66(4) 3_455 3 ?
F2 Cs1 F1 53.98(4) 1_545 3 ?
F2 Cs1 F1 102.97(4) 26_445 3 ?
F2 Cs1 F1 143.224(19) 27 3 ?
F2 Cs1 F1 143.224(19) 25_455 3 ?
F1 Cs1 F1 59.83(5) 2 3 ?
F2 Cs1 F1 113.66(4) 2 . ?
F2 Cs1 F1 53.98(4) . . ?
F2 Cs1 F1 89.50(3) 3 . ?
F2 Cs1 F1 53.98(4) 2_665 . ?
F2 Cs1 F1 89.50(3) 3_455 . ?
F2 Cs1 F1 113.66(4) 1_545 . ?
F2 Cs1 F1 143.224(19) 26_445 . ?
F2 Cs1 F1 102.97(4) 27 . ?
F2 Cs1 F1 143.223(19) 25_455 . ?
F1 Cs1 F1 59.83(5) 2 . ?
F1 Cs1 F1 59.83(5) 3 . ?
F2 Cs2 F2 74.08(5) 1_655 3 ?
F2 Cs2 F2 74.08(5) 1_655 2_665 ?
F2 Cs2 F2 74.08(5) 3 2_665 ?
F2 Cs2 F1 94.59(3) 1_655 2_655 ?
F2 Cs2 F1 56.57(4) 3 2_655 ?
F2 Cs2 F1 130.48(4) 2_665 2_655 ?
F2 Cs2 F1 56.57(4) 1_655 1_655 ?
F2 Cs2 F1 94.59(3) 3 1_655 ?
F2 Cs2 F1 130.48(4) 2_665 1_655 ?
F1 Cs2 F1 63.16(6) 2_655 1_655 ?
F2 Cs2 F1 130.48(4) 1_655 3 ?
F2 Cs2 F1 56.57(4) 3 3 ?
F2 Cs2 F1 94.59(3) 2_665 3 ?
F1 Cs2 F1 56.38(6) 2_655 3 ?
F1 Cs2 F1 119.322(8) 1_655 3 ?
F2 Cs2 F1 56.57(4) 1_655 3_665 ?
F2 Cs2 F1 130.48(4) 3 3_665 ?
F2 Cs2 F1 94.59(3) 2_665 3_665 ?
F1 Cs2 F1 119.322(8) 2_655 3_665 ?
F1 Cs2 F1 56.38(6) 1_655 3_665 ?
F1 Cs2 F1 169.91(6) 3 3_665 ?
F2 Cs2 F1 130.48(4) 1_655 . ?
F2 Cs2 F1 94.59(3) 3 . ?
F2 Cs2 F1 56.57(4) 2_665 . ?
F1 Cs2 F1 119.322(8) 2_655 . ?
F1 Cs2 F1 169.91(6) 1_655 . ?
F1 Cs2 F1 63.16(6) 3 . ?
F1 Cs2 F1 119.322(8) 3_665 . ?
F2 Cs2 F1 94.59(3) 1_655 2_665 ?
F2 Cs2 F1 130.48(4) 3 2_665 ?
F2 Cs2 F1 56.57(4) 2_665 2_665 ?
F1 Cs2 F1 169.91(6) 2_655 2_665 ?
F1 Cs2 F1 119.322(8) 1_655 2_665 ?
F1 Cs2 F1 119.322(8) 3 2_665 ?
F1 Cs2 F1 63.16(6) 3_665 2_665 ?
F1 Cs2 F1 56.38(6) . 2_665 ?
F2 Cs2 F1 115.25(4) 1_655 21_655 ?
F2 Cs2 F1 115.25(4) 3 21_655 ?
F2 Cs2 F1 167.80(4) 2_665 21_655 ?
F1 Cs2 F1 58.81(5) 2_655 21_655 ?
F1 Cs2 F1 58.81(5) 1_655 21_655 ?
F1 Cs2 F1 85.07(3) 3 21_655 ?
F1 Cs2 F1 85.07(3) 3_665 21_655 ?
F1 Cs2 F1 113.14(2) . 21_655 ?
F1 Cs2 F1 113.14(2) 2_665 21_655 ?
F2 Cs2 F1 167.80(4) 1_655 20 ?
F2 Cs2 F1 115.25(4) 3 20 ?
F2 Cs2 F1 115.25(4) 2_665 20 ?
F1 Cs2 F1 85.07(3) 2_655 20 ?
F1 Cs2 F1 113.14(2) 1_655 20 ?
F1 Cs2 F1 58.81(5) 3 20 ?
F1 Cs2 F1 113.14(2) 3_665 20 ?
F1 Cs2 F1 58.81(5) . 20 ?
F1 Cs2 F1 85.07(3) 2_665 20 ?
F1 Cs2 F1 54.42(5) 21_655 20 ?
F2 Cs2 F1 115.25(4) 1_655 19_665 ?
F2 Cs2 F1 167.80(4) 3 19_665 ?
F2 Cs2 F1 115.25(4) 2_665 19_665 ?
F1 Cs2 F1 113.14(2) 2_655 19_665 ?
F1 Cs2 F1 85.07(3) 1_655 19_665 ?
F1 Cs2 F1 113.14(2) 3 19_665 ?
F1 Cs2 F1 58.81(5) 3_665 19_665 ?
F1 Cs2 F1 85.07(3) . 19_665 ?
F1 Cs2 F1 58.81(5) 2_665 19_665 ?
F1 Cs2 F1 54.42(5) 21_655 19_665 ?
F1 Cs2 F1 54.42(5) 20 19_665 ?
F2 Mg1 F2 81.49(7) . 3_565 ?
F2 Mg1 F2 81.49(7) . 2_665 ?
F2 Mg1 F2 81.49(7) 3_565 2_665 ?
F2 Mg1 F2 180.0 . 25_565 ?
F2 Mg1 F2 98.51(7) 3_565 25_565 ?
F2 Mg1 F2 98.51(7) 2_665 25_565 ?
F2 Mg1 F2 98.51(7) . 27 ?
F2 Mg1 F2 179.998(1) 3_565 27 ?
F2 Mg1 F2 98.51(7) 2_665 27 ?
F2 Mg1 F2 81.49(7) 25_565 27 ?
F2 Mg1 F2 98.51(7) . 26_455 ?
F2 Mg1 F2 98.51(7) 3_565 26_455 ?
F2 Mg1 F2 180.0 2_665 26_455 ?
F2 Mg1 F2 81.49(7) 25_565 26_455 ?
F2 Mg1 F2 81.49(7) 27 26_455 ?
F1 Mg2 F1 96.71(8) 3_565 . ?
F1 Mg2 F1 96.71(8) 3_565 2_665 ?
F1 Mg2 F1 96.71(8) . 2_665 ?
F1 Mg2 F2 92.28(5) 3_565 3_565 ?
F1 Mg2 F2 166.45(10) . 3_565 ?
F1 Mg2 F2 92.28(5) 2_665 3_565 ?
F1 Mg2 F2 92.28(5) 3_565 . ?
F1 Mg2 F2 92.28(5) . . ?
F1 Mg2 F2 166.45(10) 2_665 . ?
F2 Mg2 F2 77.20(8) 3_565 . ?
F1 Mg2 F2 166.45(10) 3_565 2_665 ?
F1 Mg2 F2 92.28(5) . 2_665 ?
F1 Mg2 F2 92.28(5) 2_665 2_665 ?
F2 Mg2 F2 77.20(8) 3_565 2_665 ?
F2 Mg2 F2 77.20(8) . 2_665 ?
F1 Ca1 F1 180.00(7) 19 . ?
F1 Ca1 F1 92.73(6) 19 21 ?
F1 Ca1 F1 87.27(6) . 21 ?
F1 Ca1 F1 87.27(6) 19 3 ?
F1 Ca1 F1 92.73(6) . 3 ?
F1 Ca1 F1 180.00(7) 21 3 ?
F1 Ca1 F1 92.73(6) 19 20 ?
F1 Ca1 F1 87.27(6) . 20 ?
F1 Ca1 F1 92.73(6) 21 20 ?
F1 Ca1 F1 87.27(6) 3 20 ?
F1 Ca1 F1 87.27(6) 19 2 ?
F1 Ca1 F1 92.73(6) . 2 ?
F1 Ca1 F1 87.27(6) 21 2 ?
F1 Ca1 F1 92.73(6) 3 2 ?
F1 Ca1 F1 180.00(8) 20 2 ?
Mg2 F1 Ca1 177.05(10) . . ?
Mg2 F1 Cs2 89.07(3) . 1_455 ?
Ca1 F1 Cs2 91.19(3) . 1_455 ?
Mg2 F1 Cs2 89.07(3) . . ?
Ca1 F1 Cs2 91.19(3) . . ?
Cs2 F1 Cs2 169.91(6) 1_455 . ?
Mg2 F1 Cs2 88.49(7) . 19_665 ?
Ca1 F1 Cs2 88.56(5) . 19_665 ?
Cs2 F1 Cs2 94.93(3) 1_455 19_665 ?
Cs2 F1 Cs2 94.93(3) . 19_665 ?
Mg2 F1 Cs1 94.80(7) . . ?
Ca1 F1 Cs1 88.15(5) . . ?
Cs2 F1 Cs1 85.14(3) 1_455 . ?
Cs2 F1 Cs1 85.14(3) . . ?
Cs2 F1 Cs1 176.71(6) 19_665 . ?
Mg1 F2 Mg2 85.00(7) . . ?
Mg1 F2 Cs2 175.16(8) . 1_455 ?
Mg2 F2 Cs2 90.16(6) . 1_455 ?
Mg1 F2 Cs1 91.23(3) . . ?
Mg2 F2 Cs1 97.23(3) . . ?
Cs2 F2 Cs1 89.38(3) 1_455 . ?
Mg1 F2 Cs1 91.23(3) . 1_565 ?
Mg2 F2 Cs1 97.23(3) . 1_565 ?
Cs2 F2 Cs1 89.38(3) 1_455 1_565 ?
Cs1 F2 Cs1 165.49(6) . 1_565 ?
Mg1 F2 Cs1 90.78(6) . 25_455 ?
Mg2 F2 Cs1 175.78(8) . 25_455 ?
Cs2 F2 Cs1 94.06(5) 1_455 25_455 ?
Cs1 F2 Cs1 82.83(3) . 25_455 ?
Cs1 F2 Cs1 82.83(3) 1_565 25_455 ?

_diffrn_measured_fraction_theta_max 0.997
_diffrn_reflns_theta_full        27.56
_diffrn_measured_fraction_theta_full 0.997
_refine_diff_density_max         0.546
_refine_diff_density_min         -0.576
_refine_diff_density_rms         0.093
_database_code_depnum_ccdc_archive 'CCDC 1017082'
